DOI: 10.5061/dryad.98sf7m0tt
title: In-situ tensile test scanning electron microscopy dataset for solutionized Inconel 718

description: High-resolution Digital Image Correlation (HR-DIC) was performed on an
 Inconel 718 specimen, which was subjected to a heat treatment to form a
 fully solutionized system. In-situ measurements in the small strain regime
 were made through SEM imaging, followed by HR-DIC to extract quantitative
 representations of the strain and in-plane displacement induced by
 deformation events during plastic deformation.
description: <strong>Material: </strong>The present study
 investigated a nickel-based superalloy, Inconel 718. The Inconel 718
 material was subjected to an annealing treatment at 1050◦C for 30 minutes,
 followed by water quenching to produce a nearly random texture and a grain
 size distribution centered at 65 μm.
 <strong>Mechanical Testing: </strong>Flat
 dogbone-shaped specimens were prepared for testing with a gauge section
 measuring 1×3 mm2. Tensile loading was conducted at room temperature under
 a quasi-static strain rate using a custom 5000 N in situ load stage. The
 loading was intermittently interrupted at four points through past yield
 to acquire backscatter SEM images. Load was not removed during the SEM
 imaging. Macroscopic engineering strain was measured in situ using
 fiducial markers positioned at both ends of the gauge length, while
 macroscopic engineering stress was determined by dividing load cell output
 by the sample cross section. The points where loading was interrupted for
 detailed SEM imaging correspond to total strain levels of 0.38%, 0.62%,
 1.02%, and 1.95%. <strong>High-Resolution Digital
 Image Correlation: </strong>High-resolution digital image
 correlation measurements were conducted using a ThermoFisher Versa3D
 scanning electron microscopy (SEM) and Scios field emission gun
 system. Surface preparation for both specimens involved mechanical
 polishing with SiC papers up to 1200 grit, followed by polishing with a 3
 μm diamond suspension, and a final chemomechanical polish using 0.05 μm
 colloidal silica for 12 hours. The speckle pattern for HR-DIC was created
 using gold or silver nanoparticles. The resulting pattern had a high
 density of 60 nm nanoparticles suitable for HR-DIC measurements. High
 magnification images were captured at horizontal field widths (HFWs) of
 137 μm. Each SEM image consists of a 0.137 mm × 0.137 mm region
 discretized into 4096 × 4096 points, yielding a spacing or pixel size of
 33.4 nm. A series of 8 by 8 images were then collected to generate a
 composite image of approximately 1 mm × 1 mm in size of the sample
 gauge section. <strong>Electron Backscatter
 Diffraction: </strong>Prior to deformation, electron backscatter
 diffraction (EBSD) measurements were performed. EBSD measurements were
 performed with an<br>EDAX OIM-Hikari detector, using a step size of
 0.8 μm. Diffraction patterns were obtained with an accelerating voltage of
 20 kV, a 4 × 4 binning, and a beam current of 0.2 nA.
description: # In-situ tensile test scanning electron microscopy dataset for
 solutionized Inconel 718
 [https://doi.org/10.5061/dryad.98sf7m0tt](https://doi.org/10.5061/dryad.98sf7m0tt) ## Description of the data and file structure **Material:** The present study investigated a nickel-based superalloy, Inconel 718. The Inconel 718 material was subjected to an annealing treatment at 1050◦C for 30 minutes, followed by water quenching to produce a nearly random texture and a grain size distribution centered at 65 μm. **Mechanical Testing:** Flat dogbone-shaped specimens were prepared for testing with a gauge section measuring 1×3 mm2. Tensile loading was conducted at room temperature under a quasi-static strain rate using a custom 5000 N in situ load stage. The loading was intermittently interrupted at four points through past yield to acquire backscatter SEM images. Load was not removed during the SEM imaging. Macroscopic engineering strain was measured in situ using fiducial markers positioned at both ends of the gauge length, while macroscopic engineering stress was determined by dividing load cell output by the sample cross section. The points where loading was interrupted for detailed SEM imaging correspond to total strain levels of 0.38%, 0.62%, 1.02%, and 1.95%. **High-Resolution Digital Image Correlation:** High-resolution digital image correlation measurements were conducted using a ThermoFisher Versa3D scanning electron microscopy (SEM) and Scios field emission gun system. Surface preparation for both specimens involved mechanical polishing with SiC papers up to 1200 grit, followed by polishing with a 3 μm diamond suspension, and a final chemomechanical polish using 0.05 μm colloidal silica for 12 hours. The speckle pattern for HR-DIC was created using gold or silver nanoparticles. The resulting pattern had a high density of 60 nm nanoparticles suitable for HR-DIC measurements. High magnification images were captured at horizontal field widths (HFWs) of 137 μm. Each SEM image consists of a 0.137 mm × 0.137 mm region discretized into 4096 × 4096 points, yielding a spacing or pixel size of 33.4 nm. A series of 8 by 8 images were then collected to generate a composite image of approximately 1 mm × 1 mm in size of the sample gauge section. **Electron Backscatter Diffraction:** Prior to deformation, electron backscatter diffraction (EBSD) measurements were performed. EBSD measurements were performed with an EDAX OIM-Hikari detector, using a step size of 0.8 μm. Diffraction patterns were obtained with an accelerating voltage of 20 kV, a 4 × 4 binning, and a beam current of 0.2 nA. ### Files and variables #### File: EBSD\_SS.tif **Description:** This is the inverse pole figure (IPF) map along the loading direction (horizontal) for the investigated material prior to deformation. #### File: 718\_SS.ang **Description:** This is the .ang file corresponding to the EBSD data collected prior to deformation. #### File: 718\_SS\_SEM\_Images.zip **Description:** This file contains five folders containing raw SEM images before and after deformation for the investigated material. The images are 16 bit tiff images. Imaging was done on an 8x8 grid and the images have been named accordingly. The filename for every image ends with Py*_*x.tif.tif, where y_x indicates the grid position of the given image. Images before deformation are contained in the step0 folder. Images for subsequent deformation steps can be found in folders named as step1, step2, step3 and step4. The images can be registered and processed through any conventional or advanced DIC software to generate full field maps. ## Code/software SEM images can be opened using any image analysis software such as ImageJ. The EBSD .ang file can be opened using OIM analysis. It can also be opened as a standard text file using Notepad.